LMucko/crystallography-open-database huggingface dataset:
Crystal structure of alpha-Ag V O3 and phase relation of Ag V O3
Akashi, H.; Kittaka, S.; Matsuno, K.; Journal of Solid State Chemistry 142 (1999) 360–367; doi:10.1006/jssc.1998.8044

data_1509498
_publ_section_title
;
 Crystal structure of alpha-Ag V O3 and phase relation of Ag V O3
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              360
_journal_page_last               367
_journal_paper_doi               10.1006/jssc.1998.8044
_journal_volume                  142
_journal_year                    1999
_chemical_formula_sum            'Ag O3 V'
_chemical_name_systematic        'Ag (V O3)'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 99.69
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   10.437
_cell_length_b                   9.897
_cell_length_c                   5.532
_cell_volume                     563.275
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            silver1-2_477.cif
_cod_data_source_block           Ag1O3V1
_cod_original_cell_volume        563.2753
_cod_original_formula_sum        'Ag1 O3 V1'
_cod_database_code               1509498
Crystal structures and crystal chemistry of Ag X P O4 (X= Be, Zn)
Barbier, J.; Hammond, R.P.; Gallardo, C.; Journal of Solid State Chemistry 141 (1998) 177–185; doi:10.1006/jssc.1998.7942

data_1509499
_publ_section_title
;
 Crystal structures and crystal chemistry of Ag X P O4 (X= Be, Zn)
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              177
_journal_page_last               185
_journal_paper_doi               10.1006/jssc.1998.7942
_journal_volume                  141
_journal_year                    1998
_chemical_formula_sum            'Ag O4 P Zn'
_chemical_name_systematic        'Ag (Zn P O4)'
_space_group_IT_number           173
_symmetry_space_group_name_Hall  'P 6c'
_symmetry_space_group_name_H-M   'P 63'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            8
_cell_length_a                   10.218
_cell_length_b                   10.218
_cell_length_c                   7.848
_cell_volume                     709.613
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            silver1-2_478.cif
_cod_data_source_block           Ag1O4P1Zn1
_cod_original_cell_volume        709.6129
_cod_original_formula_sum        'Ag1 O4 P1 Zn1'
_cod_database_code               1509499
Crystal structures of quenched high-temperature and annealed low-temperature modifications of AgSbOSiO4
Mill', B.V.; Belokoneva, E.L.; Zhurnal Neorganicheskoi Khimii 39 (1994) 363–369; doi:

data_1509500
_publ_section_title
;
 Crystal structures of quenched high-temperature and annealed
 low-temperature modifications of AgSbOSiO4
;
_journal_name_full               'Zhurnal Neorganicheskoi Khimii'
_journal_page_first              363
_journal_page_last               369
_journal_volume                  39
_journal_year                    1994
_chemical_formula_sum            'Ag O5 Sb Si'
_chemical_name_systematic        'Ag Sb O (Si O4)'
_space_group_IT_number           52
_symmetry_space_group_name_Hall  '-P 2n 2bc'
_symmetry_space_group_name_H-M   'P n a n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   12.781
_cell_length_b                   6.307
_cell_length_c                   10.754
_cell_volume                     866.877
_citation_journal_id_ASTM        ZNOKAQ
_cod_data_source_file            silver1-2_479.cif
_cod_data_source_block           Ag1O5Sb1Si1
_cod_original_cell_volume        866.8774
_cod_original_sg_symbol_Hall     '-P 2a 2bc (-x,z,y)'
_cod_original_formula_sum        'Ag1 O5 Sb1 Si1'
_cod_database_code               1509500
Crystal structures of beta-NaSbOGeO4 and AgSbOSiO4 and migration paths of ions in structures of KTiOPO4 type
Belokoneva, E.L.; Mill', B.V.; Zhurnal Neorganicheskoi Khimii 39 (1994) 355–362; doi:

data_1509501
_publ_section_title
;
 Crystal structures of beta-NaSbOGeO4 and AgSbOSiO4 and migration paths of
 ions in structures of KTiOPO4 type
;
_journal_name_full               'Zhurnal Neorganicheskoi Khimii'
_journal_page_first              355
_journal_page_last               362
_journal_volume                  39
_journal_year                    1994
_chemical_formula_sum            'Ag O5 Sb Si'
_chemical_name_systematic        'Ag Sb O (Si O4)'
_space_group_IT_number           33
_symmetry_space_group_name_Hall  'P 2c -2n'
_symmetry_space_group_name_H-M   'P n a 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   12.832
_cell_length_b                   6.331
_cell_length_c                   10.727
_cell_volume                     871.455
_citation_journal_id_ASTM        ZNOKAQ
_cod_data_source_file            silver1-2_480.cif
_cod_data_source_block           Ag1O5Sb1Si1
_cod_original_formula_sum        'Ag1 O5 Sb1 Si1'
_cod_database_code               1509501
X-ray structural investigation of the redistribution of silver ionsin ion-conducting channels of Ag Sb O Si O4 after annealing at various temperatures
Mill', B.V.; Belokoneva, E.L.; Zhurnal Neorganicheskoi Khimii 41 (1996) 739–746; doi:

data_1509502
_publ_section_title
;
 X-ray structural investigation of the redistribution of silver ionsin
 ion-conducting channels of Ag Sb O Si O4 after annealing at various
 temperatures
;
_journal_name_full               'Zhurnal Neorganicheskoi Khimii'
_journal_page_first              739
_journal_page_last               746
_journal_volume                  41
_journal_year                    1996
_chemical_formula_sum            'Ag O5 Sb Si'
_chemical_name_systematic        'Ag Sb O (Si O4)'
_space_group_IT_number           52
_symmetry_space_group_name_Hall  '-P 2n 2bc'
_symmetry_space_group_name_H-M   'P n a n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   12.72
_cell_length_b                   6.305
_cell_length_c                   10.728
_cell_volume                     860.381
_citation_journal_id_ASTM        ZNOKAQ
_cod_data_source_file            silver1-2_482.cif
_cod_data_source_block           Ag1O5Sb1Si1
_cod_original_cell_volume        860.3813
_cod_original_sg_symbol_Hall     '-P 2a 2bc (-x,z,y)'
_cod_original_formula_sum        'Ag1 O5 Sb1 Si1'
_cod_database_code               1509502
Crystallographic study of Ag Tl (V O3)2 a metavanadate(V) with diopside type structure
Abriel, W.; Materials Research Bulletin 21 (1986) 225–229; doi:10.1016/0025-5408(86)90210-2

data_1509503
_publ_section_title
;
 Crystallographic study of Ag Tl (V O3)2 a metavanadate(V) with diopside
 type structure
;
_journal_name_full               'Materials Research Bulletin'
_journal_page_first              225
_journal_page_last               229
_journal_paper_doi               10.1016/0025-5408(86)90210-2
_journal_volume                  21
_journal_year                    1986
_chemical_formula_sum            'Ag O6 Tl V2'
_chemical_name_systematic        'Ag Tl (V O3)2'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 102.32
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   10.736
_cell_length_b                   10.227
_cell_length_c                   5.8299
_cell_volume                     625.365
_citation_journal_id_ASTM        MRBUAC
_cod_data_source_file            silver1-2_483.cif
_cod_data_source_block           Ag1O6Tl1V2
_cod_original_cell_volume        625.3651
_cod_original_formula_sum        'Ag1 O6 Tl1 V2'
_cod_database_code               1509503
Structure cristalline de l'hexathiodimetaphosphate d'argent, Ag2 P2 S6
Khodadad, P.; Rodier, N.; Toffoli, P.; Acta Crystallographica B (24,1968-38,1982) 34 (1978) 3561–3564; doi:10.1107/S0567740878011590

data_2105351
_publ_section_title
;
 Structure cristalline de l'hexathiodimetaphosphate d'argent, Ag2 P2 S6
;
_journal_name_full               'Acta Crystallographica B (24,1968-38,1982)'
_journal_page_first              3561
_journal_page_last               3564
_journal_paper_doi               10.1107/S0567740878011590
_journal_volume                  34
_journal_year                    1978
_chemical_formula_sum            'Ag P S3'
_chemical_name_systematic        'Ag (P S3)'
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 143.1
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   11.21
_cell_length_b                   6.998
_cell_length_c                   8.972
_cell_volume                     422.595
_citation_journal_id_ASTM        ACBCAR
_cod_data_source_file            silver1-2_484.cif
_cod_data_source_block           Ag1P1S3
_cod_original_cell_volume        422.5947
_cod_original_formula_sum        'Ag1 P1 S3'
_cod_database_code               2105351
Structure du Tetrathiophosphate(V) de Zinc et d'Argent, Zn Ag P S4
Rouland, J.C.; Rodier, N.; Toffoli, P.; Khodadad, P.; Acta Crystallographica C (39,1983-) 41 (1985) 645–647; doi:

data_2018856
_publ_section_title
;
 Structure du Tetrathiophosphate(V) de Zinc et d'Argent, Zn Ag P S4
;
_journal_name_full               'Acta Crystallographica C (39,1983-)'
_journal_page_first              645
_journal_page_last               647
_journal_volume                  41
_journal_year                    1985
_chemical_formula_sum            'Ag P S4 Zn'
_chemical_name_systematic        'Zn Ag P S4'
_space_group_IT_number           33
_symmetry_space_group_name_Hall  'P 2c -2n'
_symmetry_space_group_name_H-M   'P n a 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.502
_cell_length_b                   7.599
_cell_length_c                   6.0696
_cell_volume                     576.628
_citation_journal_id_ASTM        ACSCEE
_cod_data_source_file            silver1-2_485.cif
_cod_data_source_block           Ag1P1S4Zn1
_cod_original_cell_volume        576.6284
_cod_original_formula_sum        'Ag1 P1 S4 Zn1'
_cod_database_code               2018856
ABX-Verbindungen mit Ni2In-Struktur. Darstellung und Struktur der Verbindungen Ca Cu P (As), Sr Cu P (As), Sr Ag P (As), und Eu Cu As
Mewis, A.; Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische Chemie (33,1978-41,1986) 33 (1978) 983–986; doi:

data_7209350
_publ_section_title
;
 ABX-Verbindungen mit Ni2In-Struktur. Darstellung und Struktur der
 Verbindungen Ca Cu P (As), Sr Cu P (As), Sr Ag P (As), und Eu Cu As
;
_journal_name_full
;
Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische
 Chemie (33,1978-41,1986)
;
_journal_page_first              983
_journal_page_last               986
_journal_volume                  33
_journal_year                    1978
_chemical_formula_sum            'Ag P Sr'
_chemical_name_systematic        'Ag Sr P'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   4.409
_cell_length_b                   4.409
_cell_length_c                   8.23
_cell_volume                     138.551
_citation_journal_id_ASTM        ZNBAD2
_cod_data_source_file            silver1-2_486.cif
_cod_data_source_block           Ag1P1Sr1
_cod_original_cell_volume        138.5513
_cod_original_formula_sum        'Ag1 P1 Sr1'
_cod_database_code               7209350
Darstellung,Eigenschaften und Kristallstruktur von Cu2 P7 und Strukturverfeinerungen von Cu P2 und Ag P2
Jeitschko, W.; Moeller, M.H.; Zeitschrift fuer Anorganische und Allgemeine Chemie 491 (1982) 225–236; doi:10.1002/zaac.19824910129

data_1509504
_publ_section_title
;
 Darstellung,Eigenschaften und Kristallstruktur von Cu2 P7 und
 Strukturverfeinerungen von Cu P2 und Ag P2
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              225
_journal_page_last               236
_journal_paper_doi               10.1002/zaac.19824910129
_journal_volume                  491
_journal_year                    1982
_chemical_formula_sum            'Ag P2'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 113.48
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.2167
_cell_length_b                   5.0587
_cell_length_c                   7.8059
_cell_volume                     225.157
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            silver1-2_487.cif
_cod_data_source_block           Ag1P2
_cod_original_formula_sum        'Ag1 P2'
_cod_database_code               1509504
General trends observed in the substituted thiophosphate family. Synthesis and structure of Ag Sc P2 S6 and Cd Fe P2 S6.
Lee, S.; Colombet, P.; Ouvrard, G.; Brec, R.; Inorganic Chemistry 27 (1988) 1291–1294; doi:10.1021/ic00280a041

data_4331401
_publ_section_title
;
 General trends observed in the substituted thiophosphate family.
 Synthesis and structure of Ag Sc P2 S6 and Cd Fe P2 S6.
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              1291
_journal_page_last               1294
_journal_paper_doi               10.1021/ic00280a041
_journal_volume                  27
_journal_year                    1988
_chemical_formula_sum            'Ag P2 S6 Sc'
_chemical_name_systematic        'Ag Sc (P2 S6)'
_space_group_IT_number           163
_symmetry_space_group_name_Hall  '-P 3 2c'
_symmetry_space_group_name_H-M   'P -3 1 c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   6.1736
_cell_length_b                   6.1736
_cell_length_c                   12.897
_cell_volume                     425.693
_citation_journal_id_ASTM        INOCAJ
_cod_data_source_file            silver1-2_488.cif
_cod_data_source_block           Ag1P2S6Sc1
_cod_original_cell_volume        425.6928
_cod_original_formula_sum        'Ag1 P2 S6 Sc1'
_cod_database_code               4331401
A new chain compound of vanadium (III): Ag1/2 V1/2 P S3 structure, metal ordering, and magnetic properties
Ouvrard, G.; Colombet, P.; Brec, R.; Lee, S.; Materials Research Bulletin 21 (1986) 917–928; doi:10.1016/0025-5408(86)90129-7

data_1509505
_publ_section_title
;
 A new chain compound of vanadium (III): Ag1/2 V1/2 P S3 structure, metal
 ordering, and magnetic properties
;
_journal_name_full               'Materials Research Bulletin'
_journal_page_first              917
_journal_page_last               928
_journal_paper_doi               10.1016/0025-5408(86)90129-7
_journal_volume                  21
_journal_year                    1986
_chemical_formula_sum            'Ag P2 S6 V'
_chemical_name_systematic        'Ag V (P S3)2'
_space_group_IT_number           13
_symmetry_space_group_name_Hall  '-P 2yc'
_symmetry_space_group_name_H-M   'P 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 106.62
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   6.755
_cell_length_b                   10.684
_cell_length_c                   5.921
_cell_volume                     409.469
_citation_journal_id_ASTM        MRBUAC
_cod_data_source_file            silver1-2_489.cif
_cod_data_source_block           Ag1P2S6V1
_cod_original_cell_volume        409.4688
_cod_original_formula_sum        'Ag1 P2 S6 V1'
_cod_database_code               1509505
Modification of the cationic ordering with respect to the chalcogen in the layered M M' P2 X6 phases. Synthesis and structure of two-dimensional Ag V P2 Se6
Brec, R.; Ouvrard, G.; Materials Research Bulletin 23 (1988) 1199–1209; doi:10.1016/0025-5408(88)90212-7

data_1509506
_publ_section_title
;
 Modification of the cationic ordering with respect to the chalcogen in
 the layered M M' P2 X6 phases. Synthesis and structure of two-dimensional
 Ag V P2 Se6
;
_journal_name_full               'Materials Research Bulletin'
_journal_page_first              1199
_journal_page_last               1209
_journal_paper_doi               10.1016/0025-5408(88)90212-7
_journal_volume                  23
_journal_year                    1988
_chemical_formula_sum            'Ag P2 Se6 V'
_chemical_name_systematic        'Ag V (P Se3)2'
_space_group_IT_number           5
_symmetry_space_group_name_Hall  'C 2y'
_symmetry_space_group_name_H-M   'C 1 2 1'
_cell_angle_alpha                90
_cell_angle_beta                 106.82
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   6.3399
_cell_length_b                   11.02
_cell_length_c                   6.9819
_cell_volume                     466.927
_citation_journal_id_ASTM        MRBUAC
_cod_data_source_file            silver1-2_490.cif
_cod_data_source_block           Ag1P2Se6V1
_cod_original_cell_volume        466.9268
_cod_original_formula_sum        'Ag1 P2 Se6 V1'
_cod_database_code               1509506
Structure and properties of a new family of ceramic phosphides: Ag Zn La P2, Ag Zn Sm P2, and Cu Zn Sm P2
Tejedor, P.; Stacy, A.M.; Journal of Solid State Chemistry 89 (1990) 227–236; doi:10.1016/0022-4596(90)90265-Y

data_1509507
_publ_section_title
;
 Structure and properties of a new family of ceramic phosphides: Ag Zn La
 P2, Ag Zn Sm P2, and Cu Zn Sm P2
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              227
_journal_page_last               236
_journal_paper_doi               10.1016/0022-4596(90)90265-Y
_journal_volume                  89
_journal_year                    1990
_chemical_formula_sum            'Ag P2 Sm Zn'
_chemical_name_systematic        'Ag Zn Sm P2'
_space_group_IT_number           164
_symmetry_space_group_name_Hall  '-P 3 2"'
_symmetry_space_group_name_H-M   'P -3 m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   4.1247
_cell_length_b                   4.1247
_cell_length_c                   6.692
_cell_volume                     98.599
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            silver1-2_492.cif
_cod_data_source_block           Ag1P2Sm1Zn1
_cod_original_cell_volume        98.59872
_cod_original_formula_sum        'Ag1 P2 Sm1 Zn1'
_cod_database_code               1509507
Two new thiophosphates with interlocked structures: Ag Ti2 (P S4)3 and Ag2 Nb Ti3 P6 S25
Quarton, M.; Angenault, J.; Wallez, G.; Cieren, X.; Journal of Solid State Chemistry 153 (2000) 55–65; doi:10.1006/jssc.2000.8739

data_1509508
_publ_section_title
;
 Two new thiophosphates with interlocked structures: Ag Ti2 (P S4)3 and
 Ag2 Nb Ti3 P6 S25
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              55
_journal_page_last               65
_journal_paper_doi               10.1006/jssc.2000.8739
_journal_volume                  153
_journal_year                    2000
_chemical_formula_sum            'Ag P3 S12 Ti2'
_chemical_name_systematic        'Ag Ti2 (P S4)3'
_space_group_IT_number           37
_symmetry_space_group_name_Hall  'C 2 -2c'
_symmetry_space_group_name_H-M   'C c c 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            16
_cell_length_a                   34.691
_cell_length_b                   20.018
_cell_length_c                   11.576
_cell_volume                     8038.889
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            silver1-2_493.cif
_cod_data_source_block           Ag1P3S12Ti2
_cod_original_formula_sum        'Ag1 P3 S12 Ti2'
_cod_database_code               1509508
On the Application of Phase Relationships to Complex Structures. XXIII. Automatic Determination of Crystal Structures having Pseudo-Translational Symmetry by a Modified MULTAN Procedure
Fan, H.-F.; Woolfson, M.M.; Main, P.; Yao, J.-X.; Acta Crystallographica C (39,1983-) 39 (1983) 566–569; doi:

data_2018857
_publ_section_title
;
 On the Application of Phase Relationships to Complex Structures. XXIII.
 Automatic Determination of Crystal Structures having Pseudo-Translational
 Symmetry by a Modified MULTAN Procedure
;
_journal_name_full               'Acta Crystallographica C (39,1983-)'
_journal_page_first              566
_journal_page_last               569
_journal_volume                  39
_journal_year                    1983
_chemical_formula_sum            'Ag Pb S3 Sb'
_chemical_name_systematic        'Pb Ag Sb S3'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yab'
_symmetry_space_group_name_H-M   'P 1 21/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 92.25
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.518
_cell_length_b                   12.809
_cell_length_c                   5.904
_cell_volume                     568.105
_citation_journal_id_ASTM        ACSCEE
_cod_data_source_file            silver1-2_494.cif
_cod_data_source_block           Ag1Pb1S3Sb1
_cod_original_cell_volume        568.1054
_cod_original_sg_symbol_Hall     '-P 2ybc (z,y,-x)'
_cod_original_formula_sum        'Ag1 Pb1 S3 Sb1'
_cod_database_code               2018857
Lattice parameters of R Ag Pb alloys (R=rare earth element)
Ferro, R.; Rossi, D.; Mazzone, D.; Borzone, G.; Journal of the Less-Common Metals 94 (1983) L5–L7; doi:10.1016/0022-5088(83)90162-5

data_1509509
_publ_section_title
;
 Lattice parameters of R Ag Pb alloys (R=rare earth element)
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              L5
_journal_page_last               L7
_journal_paper_doi               10.1016/0022-5088(83)90162-5
_journal_volume                  94
_journal_year                    1983
_chemical_formula_sum            'Ag Pb Yb'
_chemical_name_systematic        '(Ag Pb) Yb'
_space_group_IT_number           191
_symmetry_space_group_name_Hall  '-P 6 2'
_symmetry_space_group_name_H-M   'P 6/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   4.89
_cell_length_b                   4.89
_cell_length_c                   7.23
_cell_volume                     149.722
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            silver1-2_495.cif
_cod_data_source_block           Ag1Pb1Yb1
_cod_original_cell_volume        149.7224
_cod_original_formula_sum        'Ag1 Pb1 Yb1'
_cod_database_code               1509509